(2) U. PM. MONOTONIC AND FATIGUE PROPERTIES OF KENAF/GLASS FIBER-REINFORCED HYBRID COMPOSITES. By. ©. C. O. P. MOHAIMAN JAFFAR KASHKOL. Thesis Submitted to the School of Graduate Studies, Universiti Putra Malaysia, in Fulfilment of the Requirements for the Degree of Doctor of Philosophy. November 2016 1.
(3) All material contained within the thesis, including without limitation text, logos, icons, photographs and all other artwork, is copyright material of Universiti Putra Malaysia unless otherwise stated. Use may be made of any material contained within the thesis for non-commercial purposes from the copyright holder. Commercial use of material may only be made with the express, prior, written permission of Universiti Putra Malaysia.. ©. C. O. P. U. PM. Copyright © Universiti Putra Malaysia. 3.
(4) DEDICATION. Father & Mother. PM. Every challenging work needs self efforts as well as guidance of elders especially those who were very close to our heart. Whose affection, love, encouragement and prays of day and night make me able to get such success and honor and the reason of what I become today. My humble effort I dedicate to my sweet and loving. I am really grateful to all of you.. ©. C. O. P. You have been my inspiration, and my soul mates.. iv. U. To my sisters, my wife (Sura) and my kids (Yousif and Rahaf).
(5) Abstract of thesis presented to the Senate of Universiti Putra Malaysia in fulfilment of the requirement for the degree of Doctor of Philosophy. By. November 2016. Chairman Faculty. : :. Zulkiflle Leman, PhD Engineering. O. P. The range of applications involving natural fiber composites in engineering design is still limited due to a lack of understanding of the long-term behavior of these materials, especially under cyclic fatigue loading. The primary aim of this research was to experimentally determine the monotonic properties and fatigue life behavior of woven kenaf fiber reinforced unsaturated polyester composites and the effects of hybridization of E-glass fabric on these properties through stages of hybridization and different states of stress. This work was divided into four stages to achieve the specified objectives. The first stage investigated the mechanical properties of a single layer of woven kenaf reinforced unsaturated polyester, fabricated by vacuum infusion and hand layup. The results showed an overall improvement in tensile and flexural strengths also their corresponding moduli for composites fabricated by the hand lay-up when compared with the ones fabricated by vacuum infusion. Therefore, hand lay-up method was adopted to fabricate the hybrid composites in the next stages. The second stage focused on comparing the effect of kenaf fiber alignment on the monotonic and fatigue properties of kenaf/glass hybrid composites laminate with glass shell and kenaf core. Three types of kenaf fibers were used, namely, non-woven random mat, unidirectional twisted yarn, and plain-woven kenaf with kenaf/glass weight ratio of 30/70% and a volume fraction of 35%. Tensile, compression, flexural, and fully reversed fatigue tests were conducted. Non-woven mat kenaf hybrid composite showed the poorest properties for all tests, while woven and unidirectional kenaf displayed much higher set of properties. Hybridization with kenaf fibers improved the fatigue degradation coefficient of the final composites to 6.6% and 6.8% for woven and unidirectional kenaf, respectively, compared with 8.4% for non-woven. The third stage was continued with a partial replacement of glass fiber by woven kenaf fabric reinforced unsaturated polyester. The replacement was achieved in three weight ratios of 70/30 (H1), 55/45 (H2) and 30/70 (H3) to fabricate hybrid composites. In addition, pure glass and kenaf composites were fabricated for comparison purposes. All composites had an approximate fiber volume fraction of 35-40%. Tensile,. C ©. U. MOHAIMAN JAFFAR KASHKOL. PM. MONOTONIC AND FATIGUE PROPERTIES OF KENAF/GLASS FIBER-REINFORCED HYBRID COMPOSITES. i.
(6) PM. compression, and flexural tests were performed. Finally, the fourth stage, based on the ultimate static strength determined, uniaxial cyclic fatigue tests were conducted under three different stress ratios (R) of 0.1 (TensionTension), -1 (Tension-Compression), and 2.5 (Compression-Compression). Stress levels ranged from 30% to 70% of their ultimate static strength were used with R = 0.1 and -1, and from 40% to 90% of ultimate static strength with R = 2.5. Wohler S-N curves were generated for each stress ratio for all composites, which were used to construct a constant life diagrams for each composite. In conclusion, hybridization of glass fiber with kenaf fiber showed unique and improved influence on monotonic as well as fatigue properties.. ©. C. O. P. U. .. ii.
(7) Abstrak tesis yang dikemukakan kepada Senat Universiti Putra Malaysia sebagai memenuhi keperluan untuk ijazah Doktor Falsafah SIFAT BEREKANADA DAN KELESUAN KOMPOSIT HIBRID BERTETULANG GENTIAN KENAF/KACA. November 2016. Pengerusi Fakulti. : :. Zulkiflle Leman, PhD Kejuruteraan. O. P. Penglibatan komposit gentian semulajadi dalam bidang rekabentuk kejuruteraan masih terhad disebabkan kurang kefahaman tentang sifat jangka panjang bahan tersebut, khususnya dalam bebanan kitaran lesu. Tujuan utama penyelidikan ini adalah untuk mengkaji sifat monotonik dan kelakuan jangka hayat lesu komposit poliester tak tepu diperkuat anyaman kenaf, serta kesan hibridasi fabrik E-kaca terhadap sifat-sifat tersebut melalui peringkat hibridasi dan peringkat tegasan yang berbeza. Kajian ini dibahagikan kepada lima peringkat untuk mencapai objektif yang ditetapkan. Peringkat pertama adalah untuk mengkaji sifat mekanikal selapis anyaman komposit poliester tak tapu diperkuat gentian kenaf yang direka menggunakan infusi vakum dan teknik penekanan tanpa haba. Keputusan menunjukkan peningkatan secara keseluruhan dalam kekuatan tegangan dan lenturan, serta modulus bagi komposit yang dihasilkan secara tekanan tanpa haba. Oleh itu, kaedah tekanan tanpa haba digunakan untuk menghasilkan komposit hibrid dalam peringkat seterusnyai. Peringkat kedua memfokus kepada perbandingan kesan penjajaran gentian kenaf terhadap sifat mekanik dan kelesuan komposit hibrid kenaf/kaca berkonfigurasi selang seli bersimetri dengan petala kaca dan teras kenaf. Tiga jenis gentian kenaf digunakan iaitu alas rawak tanpa tenunan, benang pintal ekaarah dan kenaf tenunan biasa dengan nisbah berat kenaf/kaca sebanyak 30/70% serta pecahan isipadu pada 35%. Ujian tegangan, mampatan, lenturan, dan kelesuan berbalik penuh turut dijalankan. Alas tanpa tenunan hibrid kenaf diasingkan daripada perbandingan akibat kelemahan sifat dalam semua jenis ujian. Penghibridan dengan gentian kenaf berjaya meningkatkan pekali degradasi kelesuan bagi komposit terakhir, masing-masing kepada 6.6% dan 6.8% bagi kenaf tenunan dan ekaarah, dibandingkan dengan 8.4% bagi kenaf tanpa tenunan. Peringkat ketiga diteruskan dengan penggantian separa gentian kaca dengan kain kenaf tenunan diperkuat poliester tak tepu. Penggantian ini dicapai melalui tiga nisbah berat iaitu 70/30 (H1), 55/45 (H2) dan 30/70 (H3) untuk menghasilkan komposit hibrid. Selain itu, komposit kaca dan kenaf tulen turut dihasilkan untuk tujuan perbandingan. Kesemua komposit mempunyai anggaran pecahan isipadu gentian pada kadar 35-40%. Ujian tegangan, mampatan, dan. C ©. U. MOHAIMAN JAFFAR KASHKOL. PM. Oleh. iii.
(8) ©. C. O. P. U. PM. lenturan dijalankan sekali lagi. Pada peringkat keempat, berdasarkan kekuatan statik muktamad yang diperoleh pada peringkat ketiga, ujian kelesuan kitaran ekapaksi dijalankan berdasarkan tiga nisbah tegasan (R) yang berbeza iaitu pada 0.1 (Tegangan-Tegangan), -1 (TeganganMampatan), dan 2.5 (Mampatan-Mampatan). Tahap tegasan di antara 30% hingga 70% daripada kekuatan statik muktamad digunakan dengan R = 0.1 dan -1. Tahap tegasan di antara 40% hingga 90% daripada kekuatan statik muktamad dengan R = 2.5 turut digunakan. Keluk Wohler S-N dijana bagi setiap nisbah tegasan untuk semua komposit yang digunakan untuk membina gambar rajah hayat tetap untuk setiap komposit. Kesimpulannya, proses hibridasi gentian kaca dengan gentian kenaf telah menunjukkan keunikan dan pengaruh penambahbaikan terhadap sifat monotonik dan kelesuan.. iv.
(9) ACKNOWLEDGEMENTS. ©. C. O. P. U. PM. First and foremost, praise to Allah (S.W.T) for His mercy which has given me the opportunity to complete this dissertation. I would like to express my gratitude to my kind and beloved mother and father as well as my sisters for their massive support. I would like to thank my wife Sura for being patient, understanding, encouraging, and supportive in every respect, I could not have completed this journey without her. There are numerous individuals that have provided me with great support throughout the course of my PhD study, and the completion of this dissertation would not have been possible otherwise. I would like to start by thanking the chairman of my supervisory committee, Associate Professor Dr. Zulkiflle Leman and co-supervisors, Dr. Mohamed Thariq bin Hameed Sultan, Dr. Mohamad Ridzwan Ishak and Dr. Azmah Hanim Mohamed Ariff for their continuous encouragement, guidance and support throughout the duration of my study, including during the writing of my dissertation. I am especially grateful to my supervisors for providing me with the opportunity to study in the field of composite materials. I would also like to extend a special thanks to Mr. Muhammad Wildan Ilyas Mohamed Ghazali, Mr. Ahmad Shaifudin Ismail and Mr. Mohd Saiful Azuar Isa for their technical assistance during my experiments. Finally, I would like to express my gratitude and sincere appreciation to the Ministry of Higher Education & Scientific Research of Iraq for its financial support.. v.
(10) © P. O. C. U. PM.
(11) This thesis was submitted to the Senate of Universiti Putra Malaysia and has been accepted as fulfilment of the requirement for the degree of Doctor of Philosophy. The members of the Supervisory Committee were as follows:. PM. Zulkiflle Leman, PhD Associate Professor Faculty of Engineering Universiti Putra Malaysia (Chairman). U. Mohamad Ridzwan Ishak, PhD Senior Lecturer Faculty of Engineering Universiti Putra Malaysia (Member). Mohamed Thariq bin Hameed Sultan, PhD, P.Eng Associate Professor,Ir Faculty of Engineering Universiti Putra Malaysia (Member). C. O. P. Azmah Hanim Mohamed Ariff, PhD Senior Lecturer Faculty of Engineering Universiti Putra Malaysia (Member). ©. __________________________ ROBIAH BINTI YUNUS, PhD Professor and Dean School of Graduate Studies Universiti Putra Malaysia. Date:. vii.
(12) Declaration by graduate dtudent. U. PM. I hereby confirm that: x this thesis is my original work; x quotations, illustrations and citations have been duly referenced; x this thesis has not been submitted previously or concurrently for any other degree at any other institutions; x intellectual property from the thesis and copyright of thesis are fully-owned by Universiti Putra Malaysia, as according to the Universiti Putra Malaysia (Research) Rules 2012; x written permission must be obtained from supervisor and the office of Deputy Vice-Chancellor (Research and Innovation) before thesis is published (in the form of written, printed or in electronic form) including books, journals, modules, proceedings, popular writings, seminar papers, manuscripts, posters, reports, lecture notes, learning modules or any other materials as stated in the Universiti Putra Malaysia (Research) Rules 2012; x there is no plagiarism or data falsification/fabrication in the thesis, and scholarly integrity is upheld as according to the Universiti Putra Malaysia (Graduate Studies) Rules 2003 (Revision 2012-2013) and the Universiti Putra Malaysia (Research) Rules 2012. The thesis has undergone plagiarism detection software.. Signature: ________________________. Date: __________________. ©. C. O. P. Name and Matric No.: Mohaiman Jaffar Kashkol, GS38220. viii.
(13) © P. O. C. U. PM.
(14) TABLE OF CONTENTS. Page i iii v vi viii xiii xiv xix. U. PM. ABSTRACT ABSTRAK ACKNOWLEDGEMENTS APPROVAL DECLERATION LIST OF TABLES LIST OF FIGURES LIST OF ABBREVIATIONS CHAPTER INTROCUCTION 1.1 Background of Study 1.2 Problem Statement 1.3 Research Objectives 1.4 Scope of Study 1.5 Thesis Outline. 2. LITERATURE REVIEW 2.1 Introduction 2.2 Lignocellulose Kenaf Fiber 2.3 Developments of Natural Fiber Hybrid Composites Products 2.4 Natural/Synthetic Fiber Hybrid Composites 2.4.1 Monotonic properties of Kenaf /Synthetic & Lignocellulose / Glass Hybrid Composites 2.4.2 Fatigue Properties of Hybrid Composites 2.5 Factors Influencing Monotonic Properties and Fatigue Life of Hybrid Composites 2.5.1 Type and Pattern of Fiber 2.5.2 Stacking Sequence 2.5.3 Fiber Ratios 2.5.4 Fabrication Method 2.5.5 Loading Conditions and Stress Ratio 2.6 Wohler S-N Curve and Fatigue Sensitivity Coefficient 2.7 Constant Life Diagrams 2.8 Summary. ©. C. O. P. 1. 3. METHODOLOGY 3.1 Introduction 3.2 Materials 3.2.1 Kenaf 3.2.2 E-Glass 3.2.3 Unsaturated Polyester 3.3 Characterization of Woven Kenaf Fiber x. 1 1 3 4 4 5 6 6 6 8 9 10 16 20 21 23 25 28 30 33 37 38 39 39 41 41 41 42 42.
(15) 3.5 3.6. 3.7. RESULTS AND DISCUSSION 4.1 Introduction 4.2 Characterization of Kenaf Fiber 4.3 Mechanical Properties of Kenaf Composites via Different Processing Methods 4.3.1 Vacuum Infusion and Hand lay-up 4.3.2 Mechanical Properties 4.4 Monotonic and Fatigue Properties of Different Kenaf Fiber Orientation Hybrid Composites 4.4.1 Tensile Property 4.4.2 Compressive Property 4.4.3 Flexural Property 4.4.4 Fully Reversed Fatigue 4.5 Partial Replacement of Glass with Woven Kenaf Hybrid Composites 4.5.1 Tensile Property 4.5.2 Compressive Property 4.5.3 Flexural Property 4.6 Fatigue Life Assessment of Woven Kenaf/Glass Hybrid Composites under Different Fatigue Modes 4.6.1 Tension – Tension Mode 4.6.2 Tension – Compression Mode 4.6.3 Compression – Compression Mode 4.7 Constant Life Diagram and Fatigue Life Prediction 4.8 Composite Damage Mechanisms Due to Monotonic Loading 4.9 Composite Damage Mechanisms due to Fatigue Loading 4.9.1 Matrix Failure 4.9.2 Fiber Failure 4.10 Summary. ©. C. O. P. 4. U. 3.9. Fabrication of Composites 3.4.1 Vacuum Infusion 3.4.2 Hand Lay-up Density of Composites Monotonic Properties of Composites 3.6.1 Tensile Test 3.6.2 Compression Test 3.6.3 Flexural Test Determination of Fatigue Life of Hybrid Composites 3.7.1 Tension-Tension 3.7.2 Tension-Compression 3.7.3 Compression-Compression Morphological and Microscopic Observation. 43 43 44 45 46 46 47 47 48 48 49 49 50. PM. 3.4. xi. 51 51 51 52 52 53 56 57 58 60 61 66 67 68 70 73 73 77 79 82 87 91 92 92 96.
(16) 5. CONCLUSIONS AND RECOMMENDATIONS FOR FUTURE RESEARCH 5.1 Conclusions 5.2 Recommendations For Future Research. 97 99 100 118 123 124. ©. C. O. P. U. PM. REFERENCES APPENDICES BIODATA OF STUDENT LIST OF PUBLICATIONS. 97. xii.
(17) LIST OF TABLES. Table. Page Mechanical properties of the most used plant and synthetic fibers.. 8. 2.2. Reported studies on the monotonic properties, type of resin, and natural fiber pattern of kenaf/synthetic and natural/ glass reinforced thermosets and thermoplastic hybrid composites.. 13. 2.3. Reported studies on fatigue life of natural fiber and natural/synthetic hybrid reinforced polymer composites. 19. 3.1. Properties of the Reinforcements and Resin. 3.2. Designation of the First Hybrid Composites laminate. 45. 3.3. Designation of the Second Hybrid Composites laminate. 45. 4.1. Kenaf Yarns Properties. 51. 4.2. Properties of plain woven kenaf fabric. 52. 4.3. Comparison of Kenaf Reinforced Composites using Vacuum Infusion (VI) and Hand Lay-Up (HLU). 53. 4.4. Designation and Composition of the Hybrid Composites. 57. 4.5. Monotonic and Fatigue Properties of the Composites. 63. U. P. Designation and Specifications of Hybrid Composites. O. 4.6. PM. 2.1. C. 4.7. 66. Sample values of Smax/Smin for different R-values and stress levels for H1 hybrid composites. 73. Monotonic and Fatigue Properties of composites. 82. ©. 4.8. 42. xiii.
(18) LIST OF FIGURES. Figure. Page. Medical applications fabricated from fiber composites. 2. 1.2. Wind turbine blade materials specifications and prototypes fabricated from natural fiber composites. 2. 2.1. Three top hybrid configurations: (a) interlayer, (b) intra-layer and (c) intra-yarn. 10. 2.2. The degradation of composites strength until failure occurs.. 17. 2.3. Factors that influence the fatigue life of fiber-reinforced composites.. 20. 2.4. Kenaf fiber with (a) Woven, (b) Non-woven mat, and (c) Unidirectional structure.. 21. 2.5. S–N (a) and specific S–N (b) curves of woven flax and glass composites. 22. 2.6. S–N diagram for unsaturated polyester composites reinforced with different natural fibers (Where , F= Flax, J= Jute, and H= Hemp). 23. 2.7. Comparison of normalized S–N curves of hybrid and hemp fiber composites. 25. 2.8. Typical stress–strain curves of jute–polyester with variable fiber volume fraction. 27. O. P. U. PM. 1.1. S–N diagram showing fatigue life data for Jute/polyester composites with different fiber content. 28. 2.10. Block loading sequence. 30. 2.11. Constant amplitude loading for R = 0.1 with different applied mean stress and amplitude. 31. 2.12. Constant sinusoidal amplitude and types of another loading spectrum. 31. 2.13. Normalized S–N diagram showing the effect of stress ratio on fatigue life of hemp/polyester composites. Data were normalized by the UTS, and UCS. 33. ©. C. 2.9. xiv.
(19) Typical Fatigue design process of composite structures. (a) Wind turbine blade (b) Random time spectrum of material stress. (c) Block loading (d) Constant amplitude-stress waveforms. (e) Mechanical coupon testing. (f) S-N curve (g) Constant life diagram. 34. 2.15. Typical Stress-cycle curves of composites. (a) Mean stress dependency and threshold value, instructive. (b) Influence of R-ratio on glass fiber-reinforced composite, experimental data.. 36. 2.16. Principle of the constant life diagram based on S-N curve formulation.. 37. 2.17. Sketch of constant life diagram at selected N for various loading spectra.. U. 38. 2.18. Constant life diagram of glass fiber-reinforced composite.. 38. 3.1. Experimental Flowchart. 40. 3.2. Fiber Reinforcements. (a) Non-woven kenaf mat, (b) unidirectional twisted yarn kenaf, (c) plain woven E-glass, and (d) plain woven kenaf. 41. 3.3. Fabrication of composite specimen using vacuum infusion technique.. 44. 3.4. Laminate under static press. 45. 3.5. Density samples. 46. P. Samples being cut to required dimensions using circular saw. O. 3.6. PM. 2.14. Composites Specimen configuration used for: (a) Tensile, (b) Compression, and (c) Flexural Tests (all units in mm). 48. 3.8. Fatigue test specimens of (a) glass, (b), H1, (c), H2, (d), H3, and (e), kenaf laminates. 49. 3.9. (a) and (b) Typical sinusoidal constant amplitude load waveforms showing definition of terms and R-values. 50. 4.1. Comparison of Tensile and Flexural (a) strength, (b) moduli for composites using VI and HLU methods. 54. 4.2. Tensile Stress–strain curves of polymer reinforced kenaf fiber composites using HLU and VI methods.. 55. ©. C. 3.7. 47. xv.
(20) Flexural Load–extension relationship of kenaf fiber composites using different polymers types and methods. 56. 4.4. Tensile properties of composites. 58. 4.5. Compressive properties of composites. 59. 4.6. Compressive stress-strain curves of hybrid composites. 59. 4.7. Flexural properties of composites. 4.8. Flexural Load- Extension behavior of hybrid composites. 61. 4.9. S-N curves for composites fitted by power regression with R2 ≥ 0.94. The arrowheads indicate that these samples survived 1 million cycles.. 62. 4.10. Normalized S-N curves of composites. 63. 4.11. Stiffness-cycle relationships at 50% of UCS. 64. 4.12. The residual dynamic elastic modulus of specimens surviving 106 cycles. 64. 4.13. Dynamic elastic modulus and normalized number of cycles of the composites at 50% of UCS. 65. 4.14. Surface temperature variations for the composites during fatigue testing. 66. 4.15. Tensile stress- strain curves for composites. 67. PM. 4.3. Tensile strength, modulus, and elongation at break of composites. O. 4.16. P. U. 60. Compressive stress-strain curves. 69. 4.18. Compressive strength, modulus, and strain results of composites. 70. 4.19. Flexural stress-strain curves. 71. 4.20. Flexural strength, modulus, and strain results of composites. 72. 4.21. The effect of kenaf fiber ratio on the density, tensile, compressive, and flexural strength of hybrid composites. 72. ©. C. 4.17. 68. xvi.
(21) S-N curves at R=0.1 for composites showing the fatigue sensitivity coefficient (b) fitted by power law regression. The arrowheads indicate that these samples survived 1 million cycles. 73. 4.23. Normalized S-N curves of composites at R=0.1. 75. 4.24. Normalized dynamic modulus-cycle of composites during fatigue loading at 40% of UTS. 76. 4.25. Change in composites’ surface temperature during fatigue loading. 77. 4.26. S-N curves R= -1 for composites fitted by power law regression. The arrowheads indicate that these samples survived 1 million cycles. 78. 4.27. Normalized S-N curves with stiffness degradation rate for composites at R= -1. 79. 4.28. S-N curves at R=2.5 for composites fitted by power law regression. The arrowheads indicate that these samples survived 1 Million cycles. 80. 4.29. Normalized S-N curves with stiffness degradation rate for composites at R=2.5. 80. 4.30. Kenaf content influence on Fatigue Stiffness degradation Rate per decade.. 81. 4.31. Constant Life Diagram of pure glass composite. 83. Constant Life Diagram of H1 composite. O. 4.32. P. U. PM. 4.22. 4.33. Constant Life Diagram of H2 composite. 85. 4.34. Constant Life Diagram of H3 composite. 86. 4.35. Constant Life Diagram of pure kenaf composite. 87. 4.36. SEM images of tensile section failure of kenaf reinforced UP composites (a) and (b) using VI method (c) and (d) using HLU method. 88. 4.37. Micrographs of tensile failure sections of kenaf hybrid composites: (a) and (d) non-woven mat, (b) plain woven, and (c) unidirectional twisted yarns. 89. 4.38. Tensile failure surfaces of (a, b) kenaf and (c, d) H1 composites. 90. C ©. 84. xvii.
(22) Compressive fracture surfaces of (a, b) kenaf/UP and (c, d) H1 composites. 91. 4.40. Failure modes under Tension-Tension Loading of (a) glass, (b) H1, (c) H2, (d) H3, and (e) woven kenaf composites. 93. 4.41. Damage development in a woven laminate during tension– tension fatigue. 94. 4.42. Failure modes under tension-compression load of (a) pure glass, (b) unidirectional kenaf/glass, (c) non-woven kenaf mat/glass, and (d) woven kenaf /glass composites. 94. 4.43. Failure modes under Tension-Compression loading of (a) glass, (b) H1 , (c) H2 , (d) H3, and (e) woven kenaf composites. 95. 4.44. Failure modes under Compression-Compression loading of (a) glass, (b) H1 , (c) H2 , (d) H3, and (e) woven kenaf composites. 95. ©. C. O. P. U. PM. 4.39. xviii.
(23) LIST OF ABBREVIATIONS. CO2. Carbon dioxide. C-C. Compression-Compression. HLU. Hand Lay-Up. HCFS. High Cyclic Fatigue Strength. HE. Hybridization Effect. ISO. International Organization for Standardization. IRT. Infrared Radiation Thermography. NDE. Non-Destructive Examination. NWK. Non- Woven Kenaf mat. SEM. Scanning Electron Microscopy. S-N. Stress-Number of Cycles. T-T. Tension-Tension. T-C. Tension-Compression. UDK. Unidirectional Kenaf. UP. Unsaturated Polyester. UCS. Ultimate Compressive Strength. UTS. Ultimate Tensile Strength. VI. Vacuum Infusion. WK. Woven Kenaf. O C ©. xix. U. PM. American Society for Testing and Materials. P. ASTM.
(24) CHAPTER 1. INTRODUCTION. 1.1. Background of Study. U. PM. Polymer composites reinforcement fibers can commonly classify into two types: synthetic fibers such as glass, carbon, etc., and natural fibers including kenaf, flax, hemp, sisal, etc (Mohanty et al., 2000). Although the glass fiber reinforced plastic composites meet structural and durability demands, they have shortcomings such as in their relatively high fiber density, difficulty to the machine, small recycling properties, and the potential health hazards posed by glass fiber particulates (Holbery et al., 2006). Natural fibers are environmentally friendly and sustainable materials, which can be used to replace synthetic fibers in the composite industry (Faruk et al., 2014). Despite this attractiveness of natural fiber reinforcement, several disadvantages were noticed, such as poor wettability, inconsistence physical and mechanical properties, and low moisture resistance makes it insufficient for advanced applications (Abedin et al., 2006). Therefore, hybrid fibers composite is the best solution to overcome these disadvantages and create a balance in the advantages of individual ones (Faruk et al., 2014).. ©. C. O. P. In the last decade natural/ synthetic hybrid fiber composites have an increased interest due to the environmental awareness of consumers and as a realistic alternatives to replace or reduce synthetic fibers usage (Swolfs et al., 2014). This applied in many sectors for application consumer’s goods and low cost housing (Ratna and Rao 2011), structural (Atiqah et al., 2014), automotive components (Davoodi et al., 2010), military and ballistic (Yahaya et al., 2014a, 2014c), and biomedical applications like orthopedic medicine and socket prosthesis (Bagheri et al., 2013; Bharath et al.; Me et al., 2012; Ramakrishna et al., 2001; Scholz et al., 2011). Figure 1.1 and Figure 1.2 show some of the potential applications developed using natural/synthetic hybrid composites. Recently, the use of hybrid composites have found increased applications in bridges and building construction sectors (Faruk et al., 2014).. 1.
(25) PM U. P. Figure 1.1: Medical applications fabricated from fiber composites 5DPDNULVKQD6FKRO] . ©. C. O. Figure 1.2: Wind turbine blade materials specifications and prototypes fabricated from natural fiber composites 6KDK. Hybrid composites offer three key benefits over single reinforcement composites for many reasons. Firstly, they offer engineers with new choices of tailoring composites to attain required properties (Swolfs et al., 2014). Secondly, a more cost-effective use of highly cost and nonrenewable fibers as glass could be achieved by changing them partially with cheaper and ecofriendly fibers such as kenaf (Mansor et al., 2013). Finally, a balanced mixture of properties for instant, strength, ductility, and stiffness can be achieved by hybrid composites (Jawaid et al., 2011). The glass fiber is more prevalent, as it offers greater improvements in most mechanical properties. Precisely, kenaf bast fiber which has been proven using analytical hierarchy process to be the best choice for hybridization with synthetic fibers for different structural applications (Mansor et al., 2013; Yahaya et al., 2014). 2.
(26) PM. Fatigue has been recognized as a unique and independent failure process (Swolfs et al., 2014). Widespread studies of fatigue failures have led to the conclusion that fatigue causes as many as 90% (Abo-Elkhier et al., 2012) or 80% (Gassan et al., 2003) of all material failures. Although the usage of natural fibers is on the rise, around 95% of plant fibers are used for non-structural automotive components sectors (Shah et al., 2013; Swolfs et al., 2014). The fatigue performance of natural fiber composites suggests that they are suitable for use in dynamically loaded structures and may be utilized as a substitute for glass fiber reinforced composites in fatigue (Jawaid et al., 2011; Shah et al., 2013; Towo et al., 2008b).. U. However many authors assessed the fatigue life of natural fibers reinforced composites in tension–tension mode (Abdullah et al., 2015; Belaadi et al., 2013), used different fiber structure (Shah et al., 2013). A few studies were reported on the uniaxial fatigue life of hybrid (Bagheri et al., 2014; Shahzad et al., 2011; Thwe et al., 2003) which was limited to the tensile fatigue performance or for fixed fiber ratio. There are many aspects not covered yet and for an instance, the effects of the natural fiber structure of hybrid composites, the gradual replacement of synthetic fiber with natural fiber, and the fatigue stress ratio on the fatigue sensitivity and fatigue life of hybrid composites.. 1.2. Problem Statement. ©. C. O. P. Fiber-reinforced composites are drawing more concern for these weightsensitive applications due to their superior strength and stiffness is linked with low-density fibers (Swolfs et al., 2014). Extensive studies have reported tensile, flexural, low, and high-velocity impact strength of hybrid composites (Swolfs et al., 2014). The positive conclusion of these studies indicates natural fibers are good candidates to replace glass fiber composites (Ochi, 2008). However, the range of applications involving natural fiber composites in engineering design is still limited due to a lack of understanding of the longterm behavior of these materials, especially under cyclic fatigue loading. Like all composites, this can be attributed to the complex nature of how these materials fail (Fotouh et al., 2014). Also for natural fiber based composites, there has been lots of work focused on determining monotonic properties, but very limited studies related to fatigue life was observed (Fotouh et al., 2014; Shah et al., 2013).. Fatigue resistance is an essential property for many composite applications such as aircraft or wind turbine blades (Mohammed et al., 2015). The ductile fibers as natural fibers can act as crack stoppers for the broken brittle fibers as glass fiber in a hybrid composite (Swolfs et al., 2014; Hancox, 1981). Also, it is proven that natural fiber composites possess lower fatigue sensitivity than glass fiber reinforced composites (Shah et al., 2013). It could be expected to extend the fatigue life of hybrid composites compared to that of single fiber composites. 3.
(27) 1.3. PM. However, the usage of natural fiber is increased, many aspects of their behavior are still ineffectively investigated (Fotouh et al., 2014). Lack of researches regarding the fatigue behavior of kenaf or kenaf–synthetic hybrid composite, the constant life diagram is not studied yet. Hybridization influence under more complicated loading conditions such as fatigue test are not well identified. Therefore, more research is required in this area to define the essential mechanisms and to simplify the conclusions.. Research Objectives. U. The primary objective of this study to experimentally determine the monotonic properties and fatigue life behavior of woven kenaf fabric reinforced unsaturated polyester composites, also, the effects of hybridization of E-glass fabric on these properties through three stages of hybridization and different states of stress. The specific objectives of this work are: 1. 2.. 3.. 4.. Scope of Study. P. 1.4. To characterize the physical and the monotonic properties of woven kenaf fiber using vacuum infusion and hand lay-up methods. To determine the effect of kenaf fiber orientation on the monotonic properties and fatigue life of kenaf/glass-reinforced hybrid composites. To investigate the effects of partial replacement of glass by woven kenaf on monotonic and fatigue properties of kenaf/glass-reinforced hybrid composites. To determine the fatigue life of hybrid composites at different fatigue stress ratios and predicting the fatigue life cycle by generating a full constant life diagram.. ©. C. O. This study focuses on using woven textile kenaf fiber as a primary candidate, which was utilized as received without any chemical treatment. The fabrication method is an important and efficient parameter on the mechanical properties of composites. Therefore, two fabrication methods were used to fabricate a single kenaf layer reinforced unsaturated polyester fabricated using hand LayUp (HLU) and vacuum infusion (VI). Woven kenaf fiber was selected to gain the maximum performance of kenaf fiber and to replace glass fiber in hybrid composites. Hybridization was achieved via two stages. First, by fixing kenaf/glass fiber ratio and using different kenaf pattern, while the other one by changing kenaf to glass fiber ratio within the hybrid composite. The resulted hybrid composites were tested under different monotonic and fatigue loading conditions to assess the trend of; static behavior, fatigue life performance, fatigue sensitivity, failure mechanisms, and fatigue constant life diagram through hybridization process.. 4.
(28) 1.5. Thesis Outline. This research consists of five chapters including:. PM. Chapter 1: presents a brief background to the field of hybrid composite materials with focusing on the noticeable lack of mechanical behavior and highlight the research problems also, describing the objectives of research, finally defines the boundaries of this work.. U. Chapter 2: contains reviews of the available literature on natural fibers composites and factors influencing monotonic properties, cyclic fatigue loading of natural/synthetic fiber reinforced hybrid composite will be discussed in this chapter.. Chapter 3: in this chapter will show the materials specifications, mechanical tests details, equipment, and standards followed. Finally, the adopted methodology to attain the research objectives will be explained in details in this chapter. Chapter 4: discussion on the results and findings of the study will be presented in this chapter.. ©. C. O. P. Chapter 5: conclusions on the findings of the research will be drawn. Finally, the recommendations for future research will be suggested in this chapter.. 5.
(29) REFERENCES. Abdullah, A. H., Alias, S. K., Jenal, N., Abdan, K., & Ali, A. (2012). Fatigue Behavior of Kenaf Fibre Reinforced Epoxy Composites. Engineering Journal, 16(5), 105-114.. PM. Abdullah, A. H., & Mat, M. F. (2015). Fatigue Life of Arenga Pinnata/Epoxy Composites. In Advanced Materials Research (Vol. 1102, pp. 103-106). Trans Tech Publications.. U. Abedin, M., Beg, M., Pickering, K., & Khan, M. A. (2006). Study on the mechanical properties of jute/glass fiber-reinforced unsaturated polyester hybrid composites: effect of surface modification by ultraviolet radiation. Journal of Reinforced Plastics and Composites, 25(6), 575588. Abo-Elkhier, M., Hamada, A. A., & El-Deen, A. B. (2014). Prediction of fatigue life of glass fiber reinforced polyester composites using modal testing. International Journal of Fatigue, 69, 28-35. Adekunle, K., Cho, S.-W., Patzelt, C., Blomfeldt, T., & Skrifvars, M. (2011). Impact and flexural properties of flax fabrics and Lyocell fiber-reinforced bio-based thermoset. Journal of Reinforced Plastics and Composites, 0731684411405874. Afdzaluddin, A., Maleque, M. A., & Iqbal, M. (2012). Synergistic effect on flexural properties of kenaf-glass hybrid composite. Paper presented at the Advanced Materials Research. Ahmed, K. S., & Vijayarangan, S. (2008). Tensile, flexural and interlaminar shear properties of woven jute and jute-glass fabric reinforced polyester composites. Journal of materials processing technology, 207(1), 330335.. O. P. Aji, I., Zainudin, E., Khalina, A., Sapuan, S., & Khairul, M. (2011). Studying the effect of fiber size and fiber loading on the mechanical properties of hybridized kenaf/PALF-reinforced HDPE composite. Journal of Reinforced Plastics and Composites, 30(6), 546-553.. ©. C. Akil, HMl, Omar, M., Mazuki, A., Safiee, S., Ishak, Z., & Abu Bakar, A. (2011). Kenaf fiber reinforced composites: A review. Materials & Design, 32(8), 4107-4121. Akil, H. M., De Rosa, I. M., Santulli, C., & Sarasini, F. (2010). Flexural behaviour of pultruded jute/glass and kenaf/glass hybrid composites monitored using acoustic emission. Materials Science and Engineering: A, 527(12), 2942-2950. Al-Oqla, F. M., & Sapuan, S. (2014). Natural fiber reinforced polymer composites in industrial applications: feasibility of date palm fibers for sustainable automotive industry. Journal of cleaner production, 66, 347354.. 100.
(30) Alkbir, M., Sapuan, S., Nuraini, A., & Ishak, M. (2014). Effect of geometry on crashworthiness parameters of natural kenaf fibre reinforced composite hexagonal tubes. Materials & Design, 60, 85-93. Amico, S., Angrizani, C., & Drummond, M. (2008). Influence of the stacking sequence on the mechanical properties of glass/sisal hybrid composites. Journal of Reinforced Plastics and Composites.. PM. Anandjiwala, R. D., & Blouw, S. (2007). Composites from bast fibresProspects and potential in the changing market environment. Journal of Natural Fibers, 4(2), 91-109.. U. Anuar, H., Ahmad, S., Rasid, R., Ahmad, A., & Busu, W. (2008). Mechanical properties and dynamic mechanical analysis of thermoplasticǦnaturalǦ rubberǦreinforced short carbon fiber and kenaf fiber hybrid composites. Journal of applied polymer science, 107(6), 4043-4052.. Anuar, H., Ahmad, S., Rasid, R., & Daud, N. N. (2006). Tensile and impact properties of thermoplastic natural rubber reinforced short glass fiber and empty fruit bunch hybrid composites. Polymer-Plastics Technology and Engineering, 45(9), 1059-1063. Arbelaiz, A., Fernandez, B., Cantero, G., Llano-Ponte, R., Valea, A., & Mondragon, I. (2005). Mechanical properties of flax fibre/polypropylene composites. Influence of fibre/matrix modification and glass fibre hybridization. Composites Part A: applied science and manufacturing, 36(12), 1637-1644. Arthanarieswaran, V., Kumaravel, A., & Kathirselvam, M. (2014). Evaluation of mechanical properties of banana and sisal fiber reinforced epoxy composites: Influence of glass fiber hybridization. Materials & Design, 64, 194-202. ASTM. (1991). Standard Test Methods for Density and Specific Gravity (Relative Density) of Plastics by Displacement.. O. P. ASTM. (1995a). D3410-03: Standard test method for compressive properties of polymer matrix composite materials with unsupported gage section by shear loading. ASTM International.. C. ASTM. (1995b). Standard test method for tensile properties of polymer matrix composite materials. ASTM D3039/D 3039M.. ©. ASTM. (1997). Standard test Methods for Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials. ASTM. (2010). D 1895-96,“. Standard Test Methods for Apparent Density, Bulk Factor, and Pourability of Plastic Materials, 1-5. ASTM. (2012). D5229/D5229M-12" Standard Test Method for Moisture Absorption Properties and Equilibrium Conditioning of Polymer Matrix Composite Materials." ASTM International, West Conshohocken, PA, 2012. Atiqah, A., Maleque, M., Jawaid, M., & Iqbal, M. (2014). Development of kenafglass reinforced unsaturated polyester hybrid composite for structural applications. Composites Part B: Engineering, 56, 68-73. 101.
(31) Bagheri, Z. S., El Sawi, I., Bougherara, H., & Zdero, R. (2014). Biomechanical fatigue analysis of an advanced new carbon fiber/flax/epoxy plate for bone fracture repair using conventional fatigue tests and thermography. Journal of the mechanical behavior of biomedical materials, 35, 27-38.. PM. Bagheri, Z. S., El Sawi, I., Schemitsch, E. H., Zdero, R., & Bougherara, H. (2013). Biomechanical properties of an advanced new carbon/flax/epoxy composite material for bone plate applications. Journal of the mechanical behavior of biomedical materials, 20, 398406.. U. Bakar, Haznida, N., Hyie, K. M., Aidah, J., Kalam, A., & Salleh, Z. (2015). Effect of Alkaline Treatment on Tensile and Impact Strength of Kenaf/Kevlar Hybrid Composites. Paper presented at the Applied Mechanics and Materials. Bakar, M. A. A., Ahmad, S., Kuntjoro, W., & Kasolang, S. (2013). Effect of carbon fibre ratio to the impact properties of hybrid kenaf/carbon fibre reinforced epoxy composites. Paper presented at the Applied Mechanics and Materials. Bakar, N. H., Hyie, K. M., Ramlan, A. S., Hassan, M. K., & Jumahat, A. (2014). Mechanical properties of kevlar reinforcement in kenaf composites. Paper presented at the Applied Mechanics and Materials. Baker, A., & Hutchison, M. (1976). Fibre composite reinforcement of cracked aircraft structures. Aircraft Structural Fatigue, 19, 419. Basquin, O. (1910). The exponential law of endurance tests. Paper presented at the Proc. Astm. Bavan, S., & Kumar, G. M. (2010). Potential use of natural fiber composite materials in India. Journal of Reinforced Plastics and Composites, 29(24), 3600-3613.. P. Belaadi, A., Bezazi, A., Bourchak, M., & Scarpa, F. (2013). Tensile static and fatigue behaviour of sisal fibres. Materials & Design, 46, 76-83.. O. Belingardi, G., Cavatorta, M. P., & Frasca, C. (2006). Bending fatigue behavior of glass–carbon/epoxy hybrid composites. Composites Science and Technology, 66(2), 222-232.. ©. C. Bernstein, P. A., & Goodman, N. (1899, December). Approaches to concurrency control in distributed data base systems. In afips (p. 813). IEEE. Bharath, K. N., & Basavarajappa, S. (2016). Applications of biocomposite materials based on natural fibers from renewable resources: a review. Science and Engineering of Composite Materials, 23(2), 123-133. Bismarck, A., Mishra, S., & Lampke, T. (2005). Plant fibers as reinforcement for green composites. Natural fibers, biopolymers and biocomposites, 37-108. Boller, K. H. (1970). Some Fatigue Characteristics of Glass-reinforced Composite Laminates. Paper presented at the Designe News.. 102.
(32) Boopalan, M., Niranjanaa, M., & Umapathy, M. (2013). Study on the mechanical properties and thermal properties of jute and banana fiber reinforced epoxy hybrid composites. Composites Part B: Engineering, 51, 54-57. Brøndsted, P., Lilholt, H., & Lystrup, A. (2005). Composite materials for wind power turbine blades. Annu. Rev. Mater. Res., 35, 505-538.. PM. Bureau, M., & Denault, J. (2000). Fatigue behavior of continuous glass fiber composites: effect of the matrix nature. Polymer composites, 21(4), 636-644. Carvelli, V., & Lomov, S. V. (2015). Fatigue of Textile Composites: Elsevier.. U. Chang, P., Mouritz, A., & Cox, B. (2006a). Properties and failure mechanisms of pinned composite lap joints in monotonic and cyclic tension. Composites Science and Technology, 66(13), 2163-2176. Chang, P., Mouritz, A., & Cox, B. (2006b). Properties and failure mechanisms of z-pinned laminates in monotonic and cyclic tension. Composites Part A: applied science and manufacturing, 37(10), 1501-1513.. Chen, H., Miao, M., & Ding, X. (2009). Influence of moisture absorption on the interfacial strength of bamboo/vinyl ester composites. Composites Part A: applied science and manufacturing, 40(12), 2013-2019. Chow, P., Lambert, R. J., Bowers, C., & McKenzie, N. (2000). Physical and mechanical properties of composite panels made from kenaf plant fibers and plastics. Paper presented at the Proceedings of the 2000 International Kenaf Symposium, Yasuura, Hiroshima, Japan. Cicala, G., Cristaldi, G., Recca, G., Ziegmann, G., El-Sabbagh, A., & Dickert, M. (2009). Properties and performances of various hybrid glass/natural fibre composites for curved pipes. Materials & Design, 30(7), 25382542.. O. P. Coats, T. W., & Harris, C. E. (1999). A progressive damage methodology for residual strength predictions of notched composite panels. Journal of composite materials, 33(23), 2193-2224. Curtis, P. (1989). The fatigue behaviour of fibrous composite materials. The Journal of Strain Analysis for Engineering Design, 24(4), 235-244.. ©. C. DanǦMallam, Y., Abdullah, M. Z., & Yusoff, P. S. M. M. (2014). The effect of hybridization on mechanical properties of woven kenaf fiber reinforced polyoxymethylene composite. Polymer composites, 35(10), 1900-1910.. Davoodi, M., Sapuan, S., Ahmad, D., Aidy, A., Khalina, A., & Jonoobi, M. (2012). Effect of polybutylene terephthalate (PBT) on impact property improvement of hybrid kenaf/glass epoxy composite. Materials Letters, 67(1), 5-7. Davoodi, M., Sapuan, S., Ahmad, D., Ali, A., Khalina, A., & Jonoobi, M. (2010). Mechanical properties of hybrid kenaf/glass reinforced epoxy composite for passenger car bumper beam. Materials & Design, 31(10), 4927-4932.. 103.
(33) De Albuquerque, A., Joseph, K., Hecker de Carvalho, L., & d'Almeida, J. R. M. (2000). Effect of wettability and ageing conditions on the physical and mechanical properties of uniaxially oriented jute-roving-reinforced polyester composites. Composites Science and Technology, 60(6), 833-844.. PM. De Andrade Silva, F., & Mobasher, B. (2010). Fatigue behavior of sisal fiber reinforced cement composites. Materials Science and Engineering: A, 527(21), 5507-5513. De Vasconcellos, D. S., Touchard, F., & Chocinski-Arnault, L. (2014). Tension–tension fatigue behaviour of woven hemp fibre reinforced epoxy composite: A multi-instrumented damage analysis. International Journal of Fatigue, 59, 159-169.. U. Demircan, O., Yilmaz, C., Kocaman, E., Tang, S., Hamada, H., & Yildiz, M. (2015). Effect of fiber densities on impact properties of biaxial warpknitted textile composites. Journal of Reinforced Plastics and Composites, 0731684415577985. Devi, L. U., Bhagawan, S., & Thomas, S. (2010). Dynamic mechanical analysis of pineapple leaf/glass hybrid fiber reinforced polyester composites. Polymer composites, 31(6), 956-965. Dhakal, H., Zhang, Z., & Richardson, M. (2007). Effect of water absorption on the mechanical properties of hemp fibre reinforced unsaturated polyester composites. Composites Science and Technology, 67(7), 1674-1683.. Dickson, R., Fernando, G., Adam, T., Reiter, H., & Harris, B. (1989). Fatigue behaviour of hybrid composites. Journal of Materials Science, 24(1), 227-233.. O. P. Dieu, T. V., Liem, N. T., Mai, T. T., & Tung, N. H. (2004). Study on Fabrication of BMC Laminates Based on Unsaturated Polyester Resin Reinforced by Hybrid Bamboo/Glass Fibers (< Special Issue> Green Composites). JSME international journal. Series A, Solid mechanics and material engineering, 47(4), 570-573.. ©. C. Eesaee, M., & Shojaei, A. (2014). Effect of nanoclays on the mechanical properties and durability of novolac phenolic resin/woven glass fiber composite at various chemical environments. Composites Part A: applied science and manufacturing, 63, 149-158.. Emery, T. R. (2007). Identification of damage in composite materials using thermoelastic stress analysis. University of Southampton. Esfandiari, A. (2007). Mechanical properties of PP/Jute and glass fibers composites: The statistical investigation. Journal of Applied Sciences, 7(24), 3943-3950. Faruk, O., Bledzki, A. K., Fink, H.-P., & Sain, M. (2012). Biocomposites reinforced with natural fibers: 2000–2010. Progress in Polymer Science, 37(11), 1552-1596.. 104.
(34) Faruk, O., Bledzki, A. K., Fink, H. P., & Sain, M. (2014). Progress report on natural fiber reinforced composites. Macromolecular Materials and Engineering, 299(1), 9-26. Fernando, G. F. (1989). The fatigue behaviour of unidirectional mono-fibre and hybrid kevlar/xas/914 composites Thesis (Ph.D.) University of Bath (United Kingdom).. PM. Fiore, V., Di Bella, G., & Valenza, A. (2011). Glass–basalt/epoxy hybrid composites for marine applications. Materials & Design, 32(4), 20912099. Fiore, V., Di Bella, G., & Valenza, A. (2015). The effect of alkaline treatment on mechanical properties of kenaf fibers and their epoxy composites. Composites Part B: Engineering, 68, 14-21.. U. Fotouh, A., Wolodko, J. D., & Lipsett, M. G. (2014). Fatigue of natural fiber thermoplastic composites. Composites Part B: Engineering, 62, 175182. Fu, S.Y., Xu, G., & Mai, Y.-W. (2002). On the elastic modulus of hybrid particle/short-fiber/polymer composites. Composites Part B: Engineering, 33(4), 291-299. Fulton, I. T. (2011). The effect of layup and pressure on mechanical properties of fiberglass and kenaf fiber composites: Mississippi State University. Gagel, A., Lange, D., & Schulte, K. (2006). On the relation between crack densities, stiffness degradation, and surface temperature distribution of tensile fatigue loaded glass-fibre non-crimp-fabric reinforced epoxy. Composites Part A: applied science and manufacturing, 37(2), 222228.. P. Gassan, & Dietz, T. (2003). Load-increasing fatigue test to characterize the interface of composites under fatigue loadings. Journal of Materials Science, 38(12), 2755-2760.. O. Gassan, J., & Bledzki, A. K. (1999). Possibilities for improving the mechanical properties of jute/epoxy composites by alkali treatment of fibres. Composites Science and Technology, 59(9), 1303-1309.. ©. C. Guideline, G. W. (2010). Guideline for the certification of Wind Turbines. Hamburg: Germanischer Lloyd Wind Energie Gmb H. Ghani, M., Salleh, Z., Hyie, K. M., Berhan, M., Taib, Y., & Bakri, M. (2012). Mechanical properties of kenaf/fiberglass polyester hybrid composite. Procedia Engineering, 41, 1654-1659. Gheorghiu, C., Labossière, P., & Proulx, J. (2006). Fatigue and monotonic strength of RC beams strengthened with CFRPs. Composites Part A: applied science and manufacturing, 37(8), 1111-1118. Goodman, J. (1899). Mechanics applied to engineering. Longmans, Green, Chicago.. 105.
(35) Gujjala, R., Ojha, S., Acharya, S., & Pal, S. (2014). Mechanical properties of woven jute–glass hybrid-reinforced epoxy composite. Journal of composite materials, 48(28), 3445-3455. Hancox, N. (1981). Fibre composite hybrid materials: Applied Science London.. PM. Haneefa, A., Bindu, P., Aravind, I., & Thomas, S. (2008). Studies on tensile and flexural properties of short banana/glass hybrid fiber reinforced polystyrene composites. Journal of composite materials, 42(15), 14711489.. Hansen, U. (1999). Damage development in woven fabric composites during tension-tension fatigue. Journal of composite materials, 33(7), 614-639.. U. Hariharan, A. B. A., & Khalil, H. A. (2005). Lignocellulose-based hybrid bilayer laminate composite: part i-studies on tensile and impact behavior of oil palm fiber-glass fiber-reinforced epoxy resin. Journal of composite materials, 39(8), 663-684. Harris, B. (2003). Fatigue in composites. Science and technology of the fatigue response of fibrereinforced plastics. Cambridge: Woodhead Publishing Ltd.. Ho, M.-p., Wang, H., Lee, J.-H., Ho, C.-k., Lau, K.-t., Leng, J., & Hui, D. (2012). Critical factors on manufacturing processes of natural fibre composites. Composites Part B: Engineering, 43(8), 3549-3562. Hojo, Masaki, Matsuda, S., Tanaka, M., Ochiai, S., & Murakami, A. (2006). Mode I delamination fatigue properties of interlayer-toughened CF/epoxy laminates. Composites Science and Technology, 66(5), 665675. Hojo, Toshihiko, Xu, Z., Yang, Y., & Hamada, H. (2014). Tensile Properties of Bamboo, Jute and Kenaf Mat-reinforced Composite. Energy Procedia, 56, 72-79.. P. Holbery, J., & Houston, D. (2006). Natural-fiber-reinforced polymer composites in automotive applications. Jom, 58(11), 80-86.. O. Ibrahim, T., & Hafeez, T. M. (2014). A study of crashworthiness characteristic of woven kenaf fabric reinforced composites tube. Universiti Tun Hussein Onn Malaysia.. ©. C. Ishak, M., Sapuan, S., Leman, Z., Rahman, M., & Anwar, U. (2012). Characterization of sugar palm (Arenga pinnata) fibres. Journal of thermal analysis and calorimetry, 109(2), 981-989. Ismail, A. E., & Aziz, M. C. A. (2015). Fatigue strength of woven kenaf fiber reinforced composites. Paper presented at the IOP Conference Series: Materials Science and Engineering. ISO, B. (2003). 13003. Fibre-reinforced plastics–determination of fatigue properties under cyclic loading conditions. British Standards International. Jawaid, & Abdul Khalil, H. (2011). Cellulosic/synthetic fibre reinforced polymer hybrid composites: A review. Carbohydrate polymers, 86(1), 1-18. 106.
(36) Jawaid, M., Khalil, H. A., & Bakar, A. A. (2011). Woven hybrid composites: tensile and flexural properties of oil palm-woven jute fibres based epoxy composites. Materials Science and Engineering: A, 528(15), 51905195.. PM. Jayabal, S., Natarajan, U., & Sathiyamurthy, S. (2011). Effect of glass hybridization and staking sequence on mechanical behaviour of interply coir–glass hybrid laminate. Bulletin of Materials Science, 34(2), 293298. John, Jacob, M., & Thomas, S. (2008). Biofibres and biocomposites. Carbohydrate polymers, 71(3), 343-364.. U. John, K, & Naidu, S. V. (2004a). Effect of fiber content and fiber treatment on flexural properties of sisal fiber/glass fiber hybrid composites. Journal of Reinforced Plastics and Composites, 23(15), 1601-1605.. John, K, & Naidu, S. V. (2004b). Sisal fiber/glass fiber hybrid composites: the impact and compressive properties. Journal of Reinforced Plastics and Composites, 23(12), 1253-1258. John, K, & Naidu, S. V. (2004c). Tensile properties of unsaturated polyesterbased sisal fiber–glass fiber hybrid composites. Journal of Reinforced Plastics and Composites, 23(17), 1815-1819. Joseph, S., Sreekala, M., Koshy, P., & Thomas, S. (2008). Mechanical properties and water sorption behavior of phenol–formaldehyde hybrid composites reinforced with banana fiber and glass fiber. Journal of applied polymer science, 109(3), 1439-1446. Joshi, S. V., Drzal, L., Mohanty, A., & Arora, S. (2004). Are natural fiber composites environmentally superior to glass fiber reinforced composites? Composites Part A: applied science and manufacturing, 35(3), 371-376.. P. Júnior, J. H. S. A., Júnior, H. L. O., Amico, S. C., & Amado, F. D. R. (2012). Study of hybrid intralaminate curaua/glass composites. Materials & Design, 42, 111-117.. C. O. Kabir, M., Wang, H., Lau, K., & Cardona, F. (2012). Chemical treatments on plant-based natural fibre reinforced polymer composites: An overview. Composites Part B: Engineering, 43(7), 2883-2892.. ©. Kalam, A., Sahari, B., Khalid, Y., & Wong, S. (2005). Fatigue behaviour of oil palm fruit bunch fibre/epoxy and carbon fibre/epoxy composites. Composite structures, 71(1), 34-44. Kar, N., Hu, Y., Barjasteh, E., & Nutt, S. (2012). Tension–tension fatigue of hybrid composite rods. Composites Part B: Engineering, 43(5), 21152124. Katogi, H., Shimamura, Y., Tohgo, K., & Fujii, T. (2012). Fatigue behavior of unidirectional jute spun yarn reinforced PLA. Advanced Composite Materials, 21(1), 1-10. Khalil, H. A., Hanida, S., Kang, C., & Fuaad, N. N. (2007). Agro-hybrid composite: The effects on mechanical and physical properties of oil 107.
(37) palm fiber (EFB)/glass hybrid reinforced polyester composites. Journal of Reinforced Plastics and Composites, 26(2), 203-218. Khalil, H. A., Kang, C., & Adawi, T. (2008). The effect of different laminations on mechanical and physical properties of hybrid composites. Journal of Reinforced Plastics and Composites.. PM. Khan, G. A., Terano, M., Gafur, M., & Alam, M. S. (2013). Studies on the mechanical properties of woven jute fabric reinforced poly (l-lactic acid) composites. Journal of King Saud University-Engineering Sciences. Khanam, N., Reddy, G. R., Raghu, K., & Naidu, S. V. (2009). Tensile, Flexural and Compressive Properties of Coir/Silk Fiber Reinfroced Hybrid Composites. Journal of Reinforced Plastics and Composites.. U. Kistaiah, N., Kiran, C. U., Reddy, G. R., & Rao, M. S. (2014). Mechanical characterization of hybrid composites: A review. Journal of Reinforced Plastics and Composites, 33(14), 1364-1372.. Kobayashi, S., Takada, K., & Nakamura, R. (2014). Processing and characterization of hemp fiber textile composites with micro-braiding technique. Composites Part A: applied science and manufacturing, 59, 1-8. Kocsis, J, & Fejes-Kozma, Z. (1994). Failure mode and damage zone development in a GMT-PP by acoustic emission and thermography. Journal of Reinforced Plastics and Composites, 13(9), 768-792. Kocsis, J. (2000). Reinforced polymer blends. Polymer blends, 2, 395. Ku, H., Wang, H., Pattarachaiyakoop, N., & Trada, M. (2011). A review on the tensile properties of natural fiber reinforced polymer composites. Composites Part B: Engineering, 42(4), 856-873.. P. Kumar, M. A., Reddy, G. R., Bharathi, Y. S., Naidu, S. V., & Naidu, V. N. P. (2010). Frictional coefficient, hardness, impact strength, and chemical resistance of reinforced sisal-glass fiber epoxy hybrid composites. Journal of composite materials.. O. Large-Toumi, B., Salvia, M., & Vincent, L. (1996). Fiber/matrix interface effect on monotonic and fatigue behavior of unidirectional carbon/epoxy composites Fiber, Matrix, and Interface Properties: ASTM International.. ©. C. Liang, S, Gning, P. B., & Guillaumat, L. (2012). A comparative study of fatigue behaviour of flax/epoxy and glass/epoxy composites. Composites Science and Technology, 72(5), 535-543.. Liang, S., Gning, P.-B., & Guillaumat, L. (2014). Properties evolution of flax/epoxy composites under fatigue loading. International Journal of Fatigue, 63, 36-45. Maldague, X. (2001). Theory and practice of infrared technology for nondestructive testing. Maleque, M. A., Afdzaluddin, A., & Iqbal, M. (2012). Flexural and impact properties of kenaf-glass hybrid composite. Paper presented at the Advanced Materials Research. 108.
(38) Mallick, P. K. (2007). Fiber-reinforced composites: materials, manufacturing, and design: CRC press. Mandell, F, J., Ashwill, T. D., Wilson, T. J., Sears, A. T., Agastra, P., . . . Samborsky, D. D. (2010). Analysis of SNL/MSU/DOE fatigue database trends for wind turbine blade materials. Retrieved from. PM. Mandell, F, J., Reed, R. M., Samborsky, D. D., & Pan, Q. (1993). Fatigue performance of wind turbine blade composite materials. Wind Energy, 14, 191-198. Mandell, & Forbes, J. (1981). Fatigue behavior of fiber-resin composites.. Mandell, J. (1990). Fatigue behavior of short fiber composite materials. Fatigue of composite materials, 4, 231-237.. U. Mansor, M. R., Sapuan, S., Zainudin, E. S., Nuraini, A., & Hambali, A. (2013). Hybrid natural and glass fibers reinforced polymer composites material selection using Analytical Hierarchy Process for automotive brake lever design. Materials & Design, 51, 484-492. Matthewson, M., & Kurkjian, C. R. (1988). Environmental effects on the static fatigue of silica optical fiber. Journal of the American Ceramic Society, 71(3), 177-183.. Masoud, S., Soudki, K., & Topper, T. (2001). CFRP-strengthened and corroded RC beams under monotonic and fatigue loads. Journal of composites for construction, 5(4), 228-236. Me, R. C., Ibrahim, R., & Tahir, P. M. (2012). Natural Based Biocomposite Material for Prosthetic Socket Fabrication. Alam Cipta, International Journal of Sustainable Tropical Design Research and Practice, 5(1). Miller, A., & Wingert, A. (1979). Fracture surface characterization of commercial graphite/epoxy systems Nondestructive Evaluation and Flaw Criticality for Composite Materials: ASTM International.. O. P. Mishra, S., Mohanty, A., Drzal, L., Misra, M., Parija, S., Nayak, S., & Tripathy, S. (2003). Studies on mechanical performance of biofibre/glass reinforced polyester hybrid composites. Composites Science and Technology, 63(10), 1377-1385.. ©. C. Mohammed, L., Ansari, M. N., Pua, G., Jawaid, M., & Islam, M. S. (2015). A review on natural fiber reinforced polymer composite and its applications. International Journal of Polymer Science, 2015. Mohanty, A., Misra, M., & Hinrichsen, G. (2000). Biofibres, biodegradable polymers and biocomposites: an overview. Macromolecular Materials and Engineering, 276(1), 1-24. Montesano, J. (2012). Fatigue damage characterization of braided and woven fiber reinforced polymer matrix composites at room and elevated temperatures. Ryerson University. Monti, A., & Alexopoulou, E. (2013). Kenaf: A Multi-Purpose Crop for Several Industrial Applications: Springer.. 109.
(39) Mu, Q., Wei, C., & Feng, S. (2009). Studies on mechanical properties of sisal fiber/phenol formaldehyde resin inǦsitu composites. Polymer composites, 30(2), 131-137. Murali Mohan Rao, K., Mohana Rao, K., & Ratna Prasad, A. (2010). Fabrication and testing of natural fibre composites: Vakka, sisal, bamboo and banana. Materials & Design, 31(1), 508-513.. PM. Naidu, V. N. P., Kumar, M. A., Reddy, G. R., Khanm, P. N., Reddy, M. M., & Chakradhar, K. (2011). Tensile & flexural properties of sisal/glass fibre reinforced hybrid composites. International Journal of Macromolecular Science, 1(1), 19-22.. U. Naidu, V. N. P., Reddy, G. R., & Kumar, M. A. (2011). Thermal conductivity of Sisal/Glass fibre reinforced hybrid composites. International Journal of Fiber and Textile Research, 1(1), 28-30. Naik, N., & Ganesh, V. (1996). Failure behavior of plain weave fabric laminates under on-axis uniaxial tensile loading: I—analytical predictions. Journal of composite materials, 30(16), 1779-1822.. Nayak, S. K., Mohanty, S., & Samal, S. K. (2010a). Hybridization effect of glass fibre on mechanical, morphological and thermal properties of polypropylene-bamboo/glass fibre hybrid composites. Polymers & polymer composites, 18(4), 205-218. Nayak, S. K., Mohanty, S., & Samal, S. K. (2010b). Influence of interfacial adhesion on the structural and mechanical behavior of PPǦ banana/glass hybrid composites. Polymer composites, 31(7), 12471257. Nijssen, R. (2006). OptiDAT–fatigue of wind turbine materials database. regularly updates via www. wmc. nl.. P. Nunna, S., Chandra, P. R., Shrivastava, S., & Jalan, A. (2012). A review on mechanical behavior of natural fiber based hybrid composites. Journal of Reinforced Plastics and Composites, 31(11), 759-769.. O. Ochi, S. (2008). Mechanical properties of kenaf fibers and kenaf/PLA composites. Mechanics of materials, 40(4), 446-452.. ©. C. Ornaghi, H. L., Bolner, A. S., Fiorio, R., Zattera, A. J., & Amico, S. C. (2010). Mechanical and dynamic mechanical analysis of hybrid composites molded by resin transfer molding. Journal of applied polymer science, 118(2), 887-896.. Owen, M., & Howe, R. (1972). The accumulation of damage in a glassreinforced plastic under tensile and fatigue loading. Journal of Physics D: Applied Physics, 5(9), 1637. Panthapulakkal, S., & Sain, M. (2007). Studies on the water absorption properties of short hemp—glass fiber hybrid polypropylene composites. Journal of composite materials, 41(15), 1871-1883. Park, R., & Jang, J. (2000). Effect of stacking sequence on the compressive performance of impacted aramid fiber/glass fiber hybrid composite. Polymer composites, 21(2), 231-237. 110.
(40) Petrucci, R., Santulli, C., Puglia, D., Sarasini, F., Torre, L., & Kenny, J. (2013). Mechanical characterisation of hybrid composite laminates based on basalt fibres in combination with flax, hemp and glass fibres manufactured by vacuum infusion. Materials & Design, 49, 728-735. Piggott, M., & Harris, B. (1981). Compression strength of hybrid fibrereinforced plastics. Journal of Materials Science, 16(3), 687-693.. PM. Pinter, G., Ladstätter, E., Billinger, W., & Lang, R. (2006). Characterisation of the tensile fatigue behaviour of RTM-laminates by isocyclic stress– strain-diagrams. International Journal of Fatigue, 28(10), 1277-1283.. U. Pothan, LA, Cherian, B., Anandakutty, B., & Thomas, S. (2007). Effect of layering pattern on the water absorption behavior of banana glass hybrid composites. Journal of applied polymer science, 105(5), 25402548. Pothan, L. A., George, C. N., John, M. J., & Thomas, S. (2010). Dynamic mechanical and dielectric behavior of banana-glass hybrid fiber reinforced polyester composites. Journal of Reinforced Plastics and Composites, 29(8), 1131-1145. Prasad, B. M., & Sain, M. M. (2003). Mechanical properties of thermally treated hemp fibers in inert atmosphere for potential composite reinforcement. Materials Research Innovations, 7(4), 231-238. Qiao, P., Yang, H.-S., & Wolcott, M. P. (2009). Flexural fatigue and reliability analysis of wood flour/high-density polyethylene composites. Journal of Reinforced Plastics and Composites. Quaresimin, M, Carraro, P., Mikkelsen, L. P., Lucato, N., Vivian, L., . . . Talreja, R. (2014). Damage evolution under cyclic multiaxial stress state: A comparative analysis between glass/epoxy laminates and tubes. Composites Part B: Engineering, 61, 282-290.. P. Quaresimin, Marino, Susmel, L., & Talreja, R. (2010). Fatigue behaviour and life assessment of composite laminates under multiaxial loadings. International Journal of Fatigue, 32(1), 2-16.. ©. C. O. Quaresimin, M. (2002). Fatigue of woven composite laminates under tensile and compressive loading. Paper presented at the Tenth European Conference on Composite Materials (ECCM 10). Rajulu, A. V., & Devi, R. R. (2007). Compressive properties of ridge gourd/phenolic composites and ridge gourd/phenolic/glass hybrid composites. Journal of Reinforced Plastics and Composites, 26(16), 1657-1664. Ramakrishna, S., Mayer, J., Wintermantel, E., & Leong, K. W. (2001). Biomedical applications of polymer-composite materials: a review. Composites Science and Technology, 61(9), 1189-1224. Ramaswamy, G. N., Sellers, T., & Tao, W. (2003). Kenaf nonwovens as substrates for laminations. Industrial Crops and Products, 17(1), 1-8.. 111.
(41) Ramesh, M., Palanikumar, K., & Reddy, K. H. (2013). Mechanical property evaluation of sisal–jute–glass fiber reinforced polyester composites. Composites Part B: Engineering, 48, 1-9. Ramnath, B. V., Kokan, S. J., Raja, R. N., Sathyanarayanan, R., Elanchezhian, C., Prasad, A. R., & Manickavasagam, V. (2013). Evaluation of mechanical properties of abaca–jute–glass fibre reinforced epoxy composite. Materials & Design, 51, 357-366.. PM. Rao, K, & Rao, K. M. (2007). Extraction and tensile properties of natural fibers: Vakka, date and bamboo. Composite structures, 77(3), 288-295. Rao, H. R., Rajulu, A. V., Reddy, G. R., & Reddy, K. H. (2009). Flexural and Compressive Properties of Bamboo and Glass Fiber Reinforced Epoxy Hybrid Composites. Journal of Reinforced Plastics and Composites.. U. Rashid, A., & Hani, A. (2013). Analysis of woven natural fiber fabrics prepared using self-designed handloom.. Rassmann, S., Paskaramoorthy, R., & Reid, R. (2011). Effect of resin system on the mechanical properties and water absorption of kenaf fibre reinforced laminates. Materials & Design, 32(3), 1399-1406. Ratim, S., Bonnia, N., & Surip, N. (2012). The effect of woven and non-woven fiber structure on mechanical properties polyester composite reinforced kenaf. Ratna Prasad, A., & Mohana Rao, K. (2011). Mechanical properties of natural fibre reinforced polyester composites: Jowar, sisal and bamboo. Materials & Design, 32(8), 4658-4663. Reddy, E. V. S., Rajulu, A. V., Reddy, K. H., & Reddy, G. R. (2010). Chemical resistance and tensile properties of glass and bamboo fibers reinforced polyester hybrid composites. Journal of Reinforced Plastics and Composites.. O. P. Reddy, G. V., Naidu, S. V., & Rani, T. S. (2008). Kapok/glass polyester hybrid composites: Tensile and hardness properties. Journal of Reinforced Plastics and Composites.. ©. C. Reddy, G. V., Rani, T. S., Rao, K. C., & Naidu, S. V. (2008). Flexural, compressive, and interlaminar shear strength properties of kapok/glass composites. Journal of Reinforced Plastics and Composites. Report, M. M. (2014). Natural Fiber Composites Market by Applications by Manufacturing Processes and by Region - Global Trends & Forecasts to 2019 (3064190). Retrieved from www.researchandmarkets.com: Rowell, R. M., Han, J. S., & Rowell, J. S. (2000). Characterization and factors effecting fiber properties. Natural Polymers and Agrofibers Bases Composites. Embrapa Instrumentacao Agropecuaria, P. O. Box 741, Sao Carlos, 13560-970 SP, Brazil, 2000., 115-134. Rowell, R. M., Sanadi, A., Jacobson, R., & Caulfield, D. (1999). Properties of kenaf/polypropylene composites. Kenaf properties, processing and products, 381.. 112.
(42) Rozman, H., Tay, G., Kumar, R., Abusamah, A., Ismail, H., & Mohd Ishak, Z. (2001). Polypropylene–oil palm empty fruit bunch–glass fibre hybrid composites: a preliminary study on the flexural and tensile properties. European Polymer Journal, 37(6), 1283-1291. Salit, M. S., Jawaid, M., Yusoff, N. B., & Hoque, M. E. (2015). Manufacturing of Natural Fibre Reinforced Polymer Composites: Springer, Cham.. PM. Salleh, Md, F., Hassan, A., Yahya, R., & Azzahari, A. D. (2014). Effects of extrusion temperature on the rheological, dynamic mechanical and tensile properties of kenaf fiber/HDPE composites. Composites Part B: Engineering, 58, 259-266.. U. Salleh, Z., Berhan, M., Hyie, K. M., & Isaac, D. (2012). Cold-pressed kenaf and fibreglass hybrid composites laminates: Effect of fibre types. Paper presented at the Proceedings of World Academy of Science, Engineering and Technology. Salleh, Z., Hyie, K. M., Berhan, M. N., Taib, Y. M., Hassan, M., & Isaac, D. (2013). Effect of low impact energy on kenaf composite and kenaf/fiberglass hybrid composite laminates. Paper presented at the Applied Mechanics and Materials. Salman, S. D., Sharba, M. J., Leman, Z., Sultan, M., Ishak, M., & Cardona, F. (2015). Physical, Mechanical, and Morphological Properties of Woven Kenaf/Polymer Composites Produced Using a Vacuum Infusion Technique. International Journal of Polymer Science, 2015.. Samborsky, D. D., Wilson, T. J., & Mandell, J. F. (2009). Comparison of tensile fatigue resistance and constant life diagrams for several potential wind turbine blade laminates. Journal of solar energy engineering, 131(1), 011006.. P. Sathishkumar, T., Naveen, J., & Satheeshkumar, S. (2014). Hybrid fiber reinforced polymer composites–a review. Journal of Reinforced Plastics and Composites, 33(5), 454-471.. ©. C. O. Scholz, M.-S., Blanchfield, J., Bloom, L., Coburn, B., Elkington, M., Fuller, J., . . . Rae, S. (2011). The use of composite materials in modern orthopaedic medicine and prosthetic devices: a review. Composites Science and Technology, 71(16), 1791-1803. Shah, , D. U., Schubel, P. J., Licence, P., & Clifford, M. J. (2012). Determining the minimum, critical and maximum fibre content for twisted yarn reinforced plant fibre composites. Composites Science and Technology, 72(15), 1909-1917.. Shah, U, D., Schubel, P. J., & Clifford, M. J. (2012). Modelling the effect of yarn twist on the tensile strength of unidirectional plant fibre yarn composites. Journal of composite materials, 0021998312440737. Shah, U, D., Schubel, P. J., Clifford, M. J., & Licence, P. (2013). Fatigue life evaluation of aligned plant fibre composites through S–N curves and constant-life diagrams. Composites Science and Technology, 74, 139149.. 113.
(43) Shah, U, D., Schubel, P. J., Licence, P., & Clifford, M. J. (2012). Hydroxyethylcellulose surface treatment of natural fibres: the new ‘twist’in yarn preparation and optimization for composites applicability. Journal of Materials Science, 47(6), 2700-2711. Shah, D. U., Schubel, P. J., & Clifford, M. J. (2013). Can flax replace E-glass in structural composites? A small wind turbine blade case study. Composites Part B: Engineering, 52, 172-181.. PM. Shahzad, & Asim. (2011). Impact and fatigue properties of hemp–glass fiber hybrid biocomposites. Journal of Reinforced Plastics and Composites, 30(16), 1389-1398.. U. Singh, B., Gupta, M., & Verma, A. (1995). Mechanical behaviour of particulate hybrid composite laminates as potential building materials. Construction and Building materials, 9(1), 39-44.. Sreekala, M., Thomas, S., & Groeninckx, G. (2005). Dynamic mechanical properties of oil palm fiber/phenol formaldehyde and oil palm fiber/glass hybrid phenol formaldehyde composites. Polymer composites, 26(3), 388-400. Srinivasan, V., Boopathy, S. R., Sangeetha, D., & Ramnath, B. V. (2014). Evaluation of mechanical and thermal properties of banana–flax based natural fibre composite. Materials & Design, 60, 620-627. Steinberger, R., Leitão, T. V., Ladstätter, E., Pinter, G., Billinger, W., & Lang, R. (2006). Infrared thermographic techniques for non-destructive damage characterization of carbon fibre reinforced polymers during tensile fatigue testing. International Journal of Fatigue, 28(10), 13401347. Stoeckel, F., Konnerth, J., & Gindl-Altmutter, W. (2013). Mechanical properties of adhesives for bonding wood—A review. International Journal of Adhesion and Adhesives, 45, 32-41.. O. P. Sukumaran, K., Satyanarayana, K., Pillai, S., & Ravikumar, K. (2001). Structure, physical and mechanical properties of plant fibers of Kerala. Metals Materials and Processes, 13(2/4), 121-136.. ©. C. Suriani, MJ, Ali, A., Khalina, A., Sapuan, S., Abdullah, S., & Haftirman. (2012). Detection of defects in natural composite materials using thermal imaging technique. Materials Testing, 54(5), 340-346. Swolfs, Y., Gorbatikh, L., & Verpoest, I. (2014). Fibre hybridisation in polymer composites: a review. Composites Part A: applied science and manufacturing, 67, 181-200.. Sørensen, B. F., & Holmes, J. W. (1996). Effect of Loading Rate on the Monotonic Tensile Behavior of a Continuous ϋ Fiber ϋ Reinforced GlassϋCeramic Matrix Composite. Journal of the American Ceramic Society, 79(2), 313-320. Talreja, R. (1981). Fatigue of composite materials: damage mechanisms and fatigue-life diagrams. Paper presented at the Proceedings of the Royal. 114.
(44) Society of London A: Mathematical, Physical and Engineering Sciences. Thakur, V. K., & Singha, A. S. (2010). Physico-chemical and mechanical characterization of natural fibre reinforced polymer composites. Iran Polym J, 19, 3-16.. PM. Thakur, V. K., & Thakur, M. K. (2014). Processing and characterization of natural cellulose fibers/thermoset polymer composites. Carbohydrate polymers, 109, 102-117.. Thakur, V. K., Thakur, M. K., & Gupta, R. K. (2014). Review: raw natural fiber– based polymer composites. International Journal of Polymer Analysis and Characterization, 19(3), 256-271.. U. Thom, H. (1998). A review of the biaxial strength of fibre-reinforced plastics. Composites Part A: applied science and manufacturing, 29(8), 869886. Thomas, S., Idicula, M., & Joseph, K. (2009). Mechanical performance of short banana/sisal hybrid fibre reinforced polyester composites. Journal of Reinforced Plastics and Composites. Thwe, M. M., & Liao, K. (2003). Durability of bamboo-glass fiber reinforced polymer matrix hybrid composites. Composites Science and Technology, 63(3), 375-387. Toubal, L., Karama, M., & Lorrain, B. (2006). Damage evolution and infrared thermography in woven composite laminates under fatigue loading. International Journal of Fatigue, 28(12), 1867-1872. Towo, A. N., & Ansell, M. P. (2008a). Fatigue evaluation and dynamic mechanical thermal analysis of sisal fibre–thermosetting resin composites. Composites Science and Technology, 68(3), 925-932.. P. Towo, A. N., & Ansell, M. P. (2008b). Fatigue of sisal fibre reinforced composites: constant-life diagrams and hysteresis loop capture. Composites Science and Technology, 68(3), 915-924.. O. Tumolva, T., Kubouchi, M., Aoki, S., & Sakai, T. (2010). Effect of fiber loading on the mechanical strength of NFR hybrid composites. ASEAN Journal of Chemical Engineering, 1, 21-26.. ©. C. Velmurugan, R., & Manikandan, V. (2007). Mechanical properties of palmyra/glass fiber hybrid composites. Composites Part A: applied science and manufacturing, 38(10), 2216-2226.. Venkata Reddy, G., Noorunnisa Khanam, P., & Shobha Rani, T. (2007). Chemical resistance studies of kapok/glass and kapok/sisal fabrics reinforced unsaturated polyester hybrid composites. Bulletin of Pure and Applied Sciences. Section C, Chemistry, 26(1). Wan Busu, W., Anuar, H., Ahmad, S., Rasid, R., & Jamal, N. (2010). The mechanical and physical properties of thermoplastic natural rubber hybrid composites reinforced with Hibiscus cannabinus, L and short glass fiber. Polymer-Plastics Technology and Engineering, 49(13), 1315-1322. 115.